phys. stat. sol. (c)**4**_{, No. 2, 418– 420 (2007) / }**DOI**_{10.1002/pssc.200673257}

© 2007 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim

## Donor impurity-related optical absorption spectra in

## GaAs-Ga

_{1}−

_{x}

## Al

_{x}

## As quantum wells: hydrostatic pressure and

## Γ

## −

## X

## conduction band mixing effects

M. E. Mora-Ramos1,2_{, S. Y. L´opez}3_{, C. A. Duque}∗4_{,}

andV. R. Velasco2

1

Facultad de Ciencias, Universidad Aut ´onoma del Estado de Morelos, Av. Universidad 1001, C.P. 62209, Cuernavaca, MOR, M´exico

2_{Inst. de Ciencia de Materiales de Madrid, CSIC, Sor Juana In´es de la Cruz 3, 28049 Madrid, Espa ˜na}
3

Fac. de Educaci´on, Universidad de Antioquia, AA 1226, Medell´ın, Colombia

4_{Inst. de F´ısica, Universidad de Antioquia, AA 1226, Medell´ın, Colombia}

Received 30 July 2006, accepted18 August 2006

Published online 7 February 2007

PACS 62.50.+p, 71.55.Eq, 73.21.Fg, 78.40.Fy, 78.67.De

Using a variational procedure within the effective mass approximation, the mixing between theΓ_{and}_{X}
conduction band valleys in GaAs-Ga1_{−}xAlxAs quantum wells is investigated by taking into account the

effect of applied hydrostatic pressure. Some optical properties such as donor and/or acceptor binding energy and impurity-related transition energies are calculated and comparisons with available experimental data are presented.

1 Introduction The effective-mass approximation (EMA) can be extended to take into account the mix-ing between theΓandX conduction-band valleys at heterointerfaces, such as GaAs-Ga1−xAlxAs. This is

done by including boundary conditions expressed in terms of an interface matrix providing a set of linear
relations between the envelope functions and their derivatives at the interface [1,2]. TheΓ−_{X} _{mixing and}
hydrostatic pressure effects in single GaAs-AlAs and double GaAs-Ga1−xAlxAs quantum wells (QW) can

be mentioned as antecedents [2, 3]. However, up to our knowledge, the study of the combined action of the
hydrostatic pressure andΓ−_{X} _{mixing on the donor and/or acceptor impurity-related transition energies}
in GaAs-Ga1−xAlxAs QWs has not been yet reported.

In this work we are presenting results of the calculation of the donor and/or acceptor binding energy and impurity-related transition energies in a GaAs-Ga1−xAlxAs QW. Calculations are performed using a

variational procedure within the effective mass approximation.

2 Theoretical framework The calculation of the states in the conduction band of the GaAs-Ga1−xAlxAs

structures is carried out inside the effective mass approximation. A model with two independent bands is employed and we limit ourselves to consider only the ground state of the system. The Hamiltonian of the system is written as [2]:

hΓ

0

0 hX

FΓ

FX

=ε

FΓ

FX

, (1)

with

hα=− ¯h 2

2mα

∂2

∂z2 −

¯

h2

2mα_{⊥}

1

ρ ∂ ∂ρ+

∂2

∂ρ2

+U(r) +εα, α= Γ,X. (2)

∗ _{Corresponding author: e-mail:}_{cduque@fisica.udea.edu.co}_{, Phone: +57-4 210 56 30, Fax: +57-4 233 01 20}

Fα

are the ΓandX related envelope-wave functions whereasεαrefers to the conduction band edge at

the pointαinkspace. The mixing of bands is introduced according to the scheme proposed by Pulsford et al. [1], in the same spirit of Ref. [2]. The boundary conditions at the interfaces are introduced via an unitary matrix that involves an adjustable phenomenological parameterγ[1]

⎡

⎢ ⎢ ⎣

FΓ

FX

∇_{F}Γ_{/m}Γ_{}
∇_{F}X_{/m}X_{}

⎤

⎥ ⎥ ⎦

Well =

⎡

⎢ ⎢ ⎣

ξ −_{γ} _{0} _{0}

+γ ξ 0 0

0 0 ξ −_{γ}

0 0 +γ ξ

⎤

⎥ ⎥ ⎦ ⎡

⎢ ⎢ ⎣

FΓ

FX

∇_{F}Γ_{/m}Γ_{}
∇_{F}X_{/m}X_{}

⎤

⎥ ⎥ ⎦

Barrier

, (3)

withξ=1−_{γ}2

. The hydrostatic pressure effects are included from the dependencies with pressure of the basic input parameters of the EMA [5]. Finally, the impurity binding energy [4] is calculated with the use of a separable trial wavefunction depending on two-variational parameters [2].

**15** **25** **35**
**10**

**11**
**12**
**13**

**15** **25** **35**
**8**

**9**
**10**
**11**

**5**
**4**
**3**
**2**
**1**

γγγγ** = 0.0**

γγγγ** = 0.3**

**(a) L = 50 Å**
**E** ** b**

** (m**

**eV**

**)**

**Pressure (kbar)**
**5**
**4**
**3**
**2**
**1**

**(b) L = 100 Å**

(A)

**0.0** **0.5** **1.0**
**9**

**10**
**11**
**12**
**13**

**0.0** **0.5** **1.0**
**7**

**8**
**9**
**10**
**11**

**P = 0**
**15 kbar**

**25 kbar**

γγγγ** = 0.0**

γγγγ** = 0.3**

**(a) L = 50 Å**
**E** **b**

** (m**

**eV**

**)**

**z _{i} (L/2)**

**P = 0**

**15 kbar**

**25 kbar**

**(b) L = 100 Å**

(B)

Fig. 1 (A)Hydrostatic pressure dependent binding energy for a donor impurity in GaAs-Ga0.7Al0.3As QWs for two

values of the QW width. Dashed lines are for zero value of theγ-mixing parameter whereas solid lines are forγ= 0_{.}3_{.}
Different impurity positions are indicated by the labels: zi = 0(1),zi = L/8(2),zi = L/4(3),zi = 3L/8(4),

andzi = L/2(5). Labels for solid lines follow the same shown sequence for the dotted cases.(B)In growth direction

impurity position dependent binding energy for a donor impurity in GaAs-Ga0.7Al0.3As QWs for several values of the

well width. Different values of the hydrostatic pressure are presented. In(A)and(B)dotted and solid lines are for zero
value of theγ-mixing parameter andγ= 0_{.}3_{, respectivel}_{y.}

3 Results and discussion In Fig. 1 we present our results for a donor binding energy as a function
of hydrostatic pressure (A) and the impurity position (B) in GaAs-Ga0.7Al0.3As QWs and considering
different configurations of the well width and theΓ−_{X} _{mixing parameter. The linear and increasing}
behavior with the pressure, for theγ = 0case, is mainly due to the diminishing of the static dielectric
constant with the pressure. For theγ= 0.3case the binding energy grows with pressure up to a maximum
(which depends of the impurity position) and then decreases due to the fact that the mixing effect induces
a decreasing of the potential barrier confining the carriers. Because of this, in the high pressure regime, the
different binding energy curves tend to the bulk hydrogenic limit for the Ga0.7Al0.3As material.

In Fig. 2 we present our results for the pressure dependent impurity related transition energy in GaAs-Ga1−xAlxAs QWs. In both cases (donor and acceptor transitions energies) we observe a quasi-linear

behavior for the low pressure. In the donor case we obtained theΓ−_{X} _{crossing where the transitions}
are from theX-GaAs minimum to the first valence confined state of the QW. Our theoretical results are

phys. stat. sol. (c)**4**_{, No. 2 (2007)} _{419}

**0**

**10**

**20**

**30**

**1.5**

**1.6**

**1.7**

**1.8**

**1.9**

**2.0**

**0**

**10**

**20**

**30**

**1.4**

**1.5**

**1.6**

**1.7**

**1.8**

**1.9**

**Donor impurity**

**Ga**

**As**

ΓΓΓΓ

**Ga**

**0.7**

**Al**

_{0.3}**As**

_{X}**(a) γγγγ = 0.3**

**200 Å**

**100 Å**

**50 Å**

**30 Å**

**L**

**L**

** = 150 Å**

**x**

**x**

** = 0.25**

**(b) γγγγ = 0.3**

**Acceptor impurity**

**Pressure (kbar)**

**En**

**er**

**g**

**y (**

**eV)**

**En**

**er**

**g**

**y (**

**eV)**

**Pressure (kbar)**

Fig. 2 Dependence of the
transition energy upon the
hydrostatic pressure in
GaAs-Ga1_{−}xAlxAs QWs. In (a)

the transitions are from the donor impurity band to the first confined valence state of the GaAs-Ga0.7Al0.3As QW. In

(b) the transitions are from the first confined conduction state of the GaAs-Ga0.75Al0.25As

QW to the acceptor impurity band. The open symbols in (b) are experimental data from Venkateswaran et al. [6].

in good agreement with available experimental findings showed in Fig. 2(b). Results can be improved by including, for example, image effects associated with the mismatch of the static dielectric constant.

4 Conclusions By using a variational procedure within the effective mass approximation, we have
inves-tigated theΓ−_{X} _{conduction band mixing and hydrostatic pressure effects on the donor and/or acceptor}
binding energy and impurity-related transition energies in GaAs-Ga1−xAlxAs QWs. We have found that

the mixing modifies in a substantial way these optical properties. Comparisons with available experimental findings shows good agreement.

Acknowledgements The authors acknowledge support from CONACYT (M´exico) and COLCIENCIAS (Colom-bia) through bilateral agreement J200.729/2004. This work has been partially supported by CODI-Universidad de Antioquia and by the Excellence Center for Novel Materials ECNM, under Colciencias contract No. 043-2005. M.E.M.R. wishes to thank Spanish Ministry of Education for support through grant SAB2004-0199.

References

[1] N. J. Pulsford, R. J. Nicholas, P. Dawson, K. J. Moore, G. Duggan, and C. T. B. Foxon, Phys. Rev. Lett.63, 2284 (1989).

[2] D. Wang, E. A. de Andrada e Silva and I. C. da Cunha Lima, Phys. Rev. B46, 7304 (1992). [3] J. H. Burnett, H. M. Cheong, W. Paul, E. S. Koteles, and B. Elman, Phys. Rev.47, 1991 (1993). [4] S. Y. L´opez, N. Porras-Montenegro, and C. A. Duque, phys. stat. sol. (c)0, 648 (2003).

[5] See: N. Raigoza, A. L. Morales, A. Montes, N. Porras-Montenegro, and C. A. Duque, Phys. Rev. B69, 045323 (2004), and references therein.

[6] U. Venkateswaran, M. Chandrasekhar, H. R. Chandrasekhar, B. A. Vojak, F. A. Chambers, and J. M. Meese, Phys. Rev. B33, 8416 (1986).

420 M. E. Mora-Raman et al.: Donor impurity-related optical absorption spectra in GaAs-Ga_{1–}*x*Al*x*As QWs